U.S. Department of Transportation
Federal Highway Administration
1200 New Jersey Avenue, SE
Washington, DC 20590
2023664000
Federal Highway Administration Research and Technology
Coordinating, Developing, and Delivering Highway Transportation Innovations
This report is an archived publication and may contain dated technical, contact, and link information 

Publication Number: FHWAHRT05062
Date: May 2007 
Users Manual for LSDYNA Concrete Material Model 159PDF Version (1.49 KB)
PDF files can be viewed with the Acrobat® Reader® Chapter 2. Theoretical ManualElastic UpdateConcrete is typically assumed to be isotropic; therefore, Hooke's Law is used for the elastic stressstrain relationship. Hooke's law depends on two elastic constants: the bulk modulus (K) and the shear modulus (G). Plastic UpdateFollowing an initial elastic phase, concrete will yield and possibly fail, depending on the state of stress (or type of test being simulated). The yield stresses are defined by a threedimensional yield surface. The functional form of the yield surface is discussed in the next section. This section briefly discusses the plasticity algorithm responsible for setting the initial yield stresses. At each time step, the stress is updated from the strain rate increments and the time step via an incremental form of Hooke's Law (an elastic increment). This updated stress is called the trial elastic stress and is denoted σ_{ij}^{T}. If the trial elastic stress state lies on or inside the yield surface, the behavior is elastic, and the plasticity algorithm is bypassed. If the trial elastic stress state lies outside the yield surface, the behavior is elasticplastic (with possible damage, hardening, and rate effects), and the plasticity algorithm returns the stress state to the yield surface. This elasticplastic stress is called the inviscid stress, and is denoted σ_{ij}^{P}. Details of the return algorithm are well documented.^{(20,21)} For those knowledgeable about plasticity, the algorithm enforces the plastic consistency condition with associated flow. For efficiency, the algorithm employs subincrementation, rather than iteration, to ensure accurate return of the stress state to the yield surface. Subincrementation is invoked when the current strain increment exceeds a maximum strain limit specified by the user, or defaulted by the model. The associative return algorithm predicts dilation of the concrete after the yield surface is engaged in the tensile and low confining pressure regimes. Modeling dilation is one reason for employing a sophisticated plasticity algorithm rather than a simple Mises return algorithm. Simple return algorithms do not model dilation. Yield SurfaceThe concrete model is a cap model with a smooth or continuous intersection between the failure surface and hardening cap. The general shape of the yield surface in the meridonal plane is shown in Figure 15 and Figure 16. This surface uses a multiplicative formulation to combine the shear (failure) surface with the hardening compaction surface (cap) smoothly and continuously. The smooth intersection eliminates the numerical complexity of treating a compressive 'corner' region between the failure surface and cap. This type of model is often referred to as a smooth cap model or as a continuous surface cap model (CSCM). Figure 15. Illustration. General shape of the concrete model yield surface in three dimensions. Figure 16. Illustration. General shape of the concrete model yield surface in two dimensions in the meridonal plane. The original formulation of the smooth cap model was developed as a function of two stress invariants.^{(22)} The developer extended the formulation to three stress invariants and verified the threeinvariant formulation by comparing smoothcap results with analytical results for the axisymmetric compression of a MohrCoulomb medium around a circular hole.^{(20,23)} The yield surface is formulated in terms of three stress invariants because an isotropic material has three independent stress invariants. The model uses J_{¢}the first invariant of the stress tensor, J′_{2}the second invariant of the deviatoric stress tensor, and _{J¢}_{3}the third invariant of the deviatoric stress tensor. The invariants are defined in terms of the deviatoric stress tensor, S_{ij} and pressure, P, as shown in Figure 17: Figure 17. Equation. Stress invariant J _{1}, J′_{2}, and J′_{3}. The three invariant yield function is based on these three invariants, and the cap hardening parameter, κ, as shown in Figure 18: Figure 18. Equation. Yield function f. Here F_{f} is the shear failure surface, F_{c} is the hardening cap, and ℜ is the Rubin threeinvariant reduction factor. Multiplying the cap ellipse function by the shear surface function allows the cap and shear surfaces to take on the same slope at their intersection, as discussed in subsequent paragraphs. Trial elastic stress invariants are temporarily updated via the trial elastic stress tensor, σ^{T}. These are denoted J_{1}^{T}, J¢_{2}^{T}, and J¢_{3}^{T}. Elastic stress states are modeled when f (J_{1}^{T}, J¢_{2}^{T}, J¢_{3}^{T}, κ^{T}) < 0. Elasticplastic stress states are modeled when f (J_{1}^{T}, J¢_{2}^{T}, J¢_{3}^{T}, κ^{T}) > 0. In this case, the plasticity algorithm returns the stress state to the yield surface so that f (J_{1}^{P}, J¢_{2}^{P}, J¢_{3}^{P}, κ^{P}) = 0. Shear Failure Surface. The strength of concrete is modeled by the shear surface in the tensile and low confining pressure regimes. The shear surface is defined along the compression meridian as shown in Figure 19: Figure 19. Equation. Shear failure surface function F_{f}. Here the values of α, β, l, q are selected by fitting the model surface to strength measurements from TXC tests conducted on plain concrete cylinders (and then adjusting these parameters to account for compaction and damage). The TXC data are typically plotted as principal stress difference versus pressure. The principal stress difference (axial stress minus confining stress) is equal to the square root of 3J¢_{2}. The shear surface is shown in Figure 20, Figure 21, and Figure 22 for typical concrete values. psi = 145.05 MPa Figure 20. Graph. Schematic of shear surface. psi = 145.05 MPa Figure 21. Graph. Schematic of twopart cap function. psi = 145.05 MPa Figure 22. Graph. Schematic of multiplicative formulation of the shear and cap surfaces. Cap Hardening Surface. The strength of concrete is modeled by a combination of the cap and shear surfaces in the low to high confining pressure regimes. More importantly, the cap is used to model plastic volume change related to pore collapse (although the pores are not explicitly modeled). The initial location of the cap determines the onset of plasticity in isotropic compression and uniaxial strain. The elliptical shape of the cap allows the onset for isotropic compression to be greater than the onset for uniaxial strain, in agreement with shear enhanced compaction data. Without ellipticity, a "flat" cap would produce identical onsets. The motion of the cap determines the shape (hardening) of the pressurevolumetric strain curves via fits with data. Without cap motion, the pressurevolumetric strain curves would be perfectly plastic. The isotropic hardening cap is a twopart function that is either unity or an ellipse, as shown in Figure 21. When the stress state is in the tensile or very low confining pressure region, the cap function is unity: yield strength via the equation in Figure 18 is independent of the cap. When the stress state is in the low to high confining pressure regimes, the cap function is an ellipse: yield strength depends on both the cap and shear surface formulations. The twopart cap function is defined as shown in Figure 23: Figure 23. Equation. Cap failure surface function F_{c}. where L(κ)is defined as shown in Figure 24: Figure 24. Equation. L of kappa. The equation in Figure 23 is equal to unity for J_{1} £ L(κ). The equation in Figure 23 describes the ellipse for J_{1} > L(κ). The intersection of the shear surface and the cap is at J_{1} = κ. κ_{0} is the value of J_{1} at the initial intersection of the cap and shear surfaces before hardening is engaged (before the cap moves). The equation in Figure 24 restrains the cap from retracting past its initial location at κ_{0}. A simpler, but less complete, way of writing the equations in Figure 23 and Figure 24 is shown in Figure 25: Figure 25. Equation. Simple cap failure surface function F_{c}. The intersection of the cap with the J_{1} axis is at J_{1} = X(κ). This intersection depends on the cap ellipticity ratio R, where R is the ratio of its major to minor axes, as shown in Figure 26: Figure 26. Equation. X as a function of kappa. The cap moves to simulate plastic volume change. The cap expands (X(κ) and κ increase) to simulate plastic volume compaction. The cap contracts (X(κ) and κ decrease) to simulate plastic volume expansion, called dilation. The motion (expansion and contraction) of the cap is based on the hardening rule, shown in Figure 27: Figure 27. Equation. Plastic volume strain ε ^{p}_{v}. Here ε ^{p}_{v} is the plastic volume strain, W is the maximum plastic volume strain, and D_{1} and D_{2} are model input parameters. X_{0} is the initial location of the cap when κ = κ_{0}. The five input parameters (X_{0}, W, D_{1}, D_{2}, and R) are obtained from fits to the pressurevolumetric strain curves in isotropic compression and uniaxial strain. X_{0} determines the pressure at which compaction initiates in isotropic compression. R, combined with X_{0}, determines the pressure at which compaction initiates in uniaxial strain. D_{1} and D_{2} determine the shape of the pressurevolumetric strain curves. W determines the maximum plastic volume compaction. Rubin Scaling Function. Concrete fails at lower values of J¢_{2} (principal stress difference) for TXE and TOR tests than it does for TXC tests conducted at the same pressure. This was previously demonstrated in Figure 1 through Figure 4. This situation indicates that concrete strength depends on the third invariant of the deviatoric stress tensor, J¢_{3}. When viewed in the deviatoric plane, a three invariant yield surface is triangular or hexagonal in shape, as shown in Figure 28. The Rubin scaling function ℜ determines the strength of concrete for any state of stress relative to the strength for TXE.^{( 24)} Strengths like TXE and TOR are simulated by scaling back the TXE shear strength by the Rubin function: ℜF_{f}. The Rubin function ℜ is a scaling function that changes the shape (radius) of the yield surface in the deviatoric plane as a function of angle as shown in Figure 28. This shape may be a circle (DruckerPrager, Maximum Octahedral Shear Stress, von Mises), a hexagon (MohrCoulomb), or an irregular hexagonlike shape (WillamWarnke) in which each of six sides is quadratic (rather than linear) between the TXC and TXE states. For comparison, a twoinvariant model cannot simultaneously model different strengths in TXC, TXE, and TOR. When viewed in the deviatoric plane, the twoinvariant yield surface is a circle, as shown in Figure 28. A twoinvariant formulation is modeled with the Rubin function equal to ℜ=1 at all angles around the circle. This means that the TXC, TOR, and TXE strengths are modeled the same. Figure 28. Illustration. Example two and threeinvariant shapes of the concrete model in the deviatoric plane. The angle is confined to the range p/6 < < p and is related to the invariants J¢_{2} and J¢_{3}, as shown in Figure 29: Figure 29. Equation. Angle beta hat in the deviatoric plane. is a normalized invariant which remains in the range 1 < < 1. For the standard laboratory tests just discussed, the values of and are shown in Figure 30: Figure 30. Equation. Relationship between beta hat and J hat. The form of the Rubin scaling function is shown in Figure 31: Figure 31. Equation. Rubin scaling function ℜ. The value of ℜ depends on the state of stress through the angle , and on experimentally determined values (fits to data) for Q_{1} and Q_{2} as functions of pressure. Strength in TOR is modeled as Q_{1}F_{f}. Strength in TXE is modeled as Q_{2}F_{f}. The Rubin threeinvariant formulation is implemented because it is more flexible in fitting data than the more commonly used WillamWarnke formulation. Four example fits of the Rubin formulation are listed below. 1. Most general fit: the shape of the yield surface in the deviatoric plane transitions with pressure from triangular, to irregular hexagonal, to circular. Input values for all eight parameters: α_{λ}, l_{1}, b_{1}, q_{1} and α_{2}, l_{2}, b_{2}, q_{2} are shown in Figure 32. Figure 32. Equation. Most general form for Q_{1} and Q_{2}. 2. MohrCoulomb fit: a straight line fit between the TXE and TXC states. The strength ratios are estimated from the MohrCoulomb friction angle ∅ as shown in Figure 33. Figure 33. Equation. MohrCoulomb form for Q_{1}, Q_{2}. 3. Twoparameter fit: the strength ratios Q_{1} and Q_{2} remain constant with pressure. Input α_{1} and α_{2}, with all other Rubin parameters set equal to zero. This allows the user to model the yield surface as an irregular (bulging) hexagonal shape in the deviator plane. 4. WillamWarnke fit: select Q_{2} as a constant or as a function of pressure. Fit Q_{1} to the WillamWarnke TOR surface, as shown in Figure 34. Figure 34. Equation. WillamWarnke form for Q_{1}. Currently, the eight input parameters, which define Q_{1} and Q_{2}, set the shape of the threeinvariant yield surface when the pressure is compressive, but not when the pressure is tensile. When the pressure is tensile, the model automatically sets Q_{1} = 0.5774 and Q_{2} = 0.5. These values simulate a triangular yield surface in the deviatoric plane, and cannot be overridden by the user. With a triangular yield surface, the strengths attained in uniaxial, equal biaxial, and equal triaxial tensile stress simulations are approximately equal. For a smooth transition between the tensile and compressive pressure regions, the user should take care to set Q_{1} = 0.5774 and Q_{2} = 0.5 at zero pressure. This is accomplished by setting α_{1}  λ_{1} = 0.5774 and α_{2}  λ_{2} = 0.5774. Damage FormulationConcrete exhibits softening (strength reduction) in the tensile and low to moderate compressive regimes. Softening is modeled via a damage formulation. Without the damage formulation, the cap model predicts perfectly plastic behavior for laboratory test simulations such as direct pull, unconfined compression, TXE, and TXE. This behavior is not realistic. Although perfectly plastic response is typical of concrete at high confining pressures, it is not representative of concrete at lower confinement and in tension. The damage formulation models both strain softening and modulus reduction. Strain softening is a decrease in strength during progressive straining after a peak strength value is reached. Modulus reduction is a decrease in the unloading/loading slopes typically observed in cyclic unload/load tests. The damage formulation is based on the work of Simo and Ju, shown in Figure 35.^{(25)} Strain softening and modulus reduction are demonstrated in psi = 145.05 MPa Figure 36 for the concrete model. Figure 35. Equation. Damaged stress σ ^{d}_{ij}. Here d is a scalar damage parameter that transforms the stress tensor without damage, denoted σ ^{vp}, into the stress tensor with damage, denoted σ ^{d}. The damage formation is applied to the stresses after they are updated by the viscoplasticity algorithm. The damage parameter d ranges from zero for no damage to 1 for complete damage. Thus 1 − d is a reduction factor whose value depends on the accumulation of damage. The effect of this reduction factor is to reduce the bulk and shear moduli isotropically (simultaneously and proportionally). Damage initiates and accumulates when strainbased energy terms exceed the damage threshold. Damage accumulation via the parameter d is based on two distinct formulations, which is called brittle damage and ductile damage. psi = 145.05 MPa Figure 36. Graph. This cap model simulation demonstrates strain softening and modulus reduction. Brittle Damage. Brittle damage accumulates when the pressure is tensile. It does not accumulate when the pressure is compressive. Brittle damage accumulation depends on the maximum principal strain, ε_{max}, as shown in Figure 37: Figure 37. Equation. Brittle damage threshold τ_{b}. Here τ _{b} is an energytype term that depends on the accumulation of total strain via ε_{max}. Brittle damage initiates when τ _{b} exceeds an initial threshold r_{0b}. Ductile Damage. Ductile damage accumulates when the pressure is compressive. It does not accumulate when the pressure is tensile. Ductile damage accumulation depends on the total strain components, ε_{ij}, as shown in Figure 38: Figure 38. Equation. Ductile damage threshold τ_{d}. Here τ_{d} is an energytype term. The stress components σ_{ij} are the elastoplastic stresses (with kinematic hardening) calculated before application of damage and rate effects. Therefore, this strainenergy term does not represent the true strain energy in the concrete. Ductile damage initiates when τ _{d} exceeds an initial threshold r_{0d}. Damage Threshold. Brittle and ductile damage initiate with plasticity. This effectively means that the initial damage surface is coincident with the plastic shear surface. Therefore, a distinct damage surface is not defined by the user. Damage initiates at peak strength on the shear surface where the plastic volume strain is dilative. Damage does not initiate on the cap where plastic volume strain is compactive. One exception to initiation of damage with initiation of plasticity is when rate effects are modeled via viscoplasticity. With viscoplasticity, the initial damage threshold is shifted (delayed), as shown in Figure 39: Figure 39. Equation. Viscoplastic damage threshold r_{0}. Here r^{s} is the damage threshold before application of viscoplasticity, and r_{0} is the shifted threshold with viscoplasticity. When η is greater than zero (rate effects are modeled), the initial damage threshold is scaled up by the term in brackets. Hence, damage initiation is delayed while plasticity accumulates. This shift requires no input parameters and is hardwired into the model based on the viscoplastic theory previously discussed. Damage accumulates when either the brittle or ductile energy term, generically called τ_{n}, exceeds the current damage threshold, r_{n}. Here the subscript 'n' indicates the nth time step. Once damage initiates, the value of the damage threshold increases. The new threshold at time step n + 1, denoted r_{n+1}, is set equal to the exceeded value of τ . If the previous value of τ did not exceed the previous threshold (an increment without damage), the threshold does not increase. Mathematically this is expressed as shown in Figure 40: Figure 40. Equation. Incremental damage threshold, small r_{n+1}. Hence each strain energy term (brittle or ductile) must increase in value above its previous maximum in order for damage to accumulate. When energy remains constant or decreases, damage temporarily stops accumulating. The description given here is effectively that of an expanding damage surface. Softening Function. As damage accumulates, the damage parameter d increases from an initial value of zero, towards a maximum value of 1. Damage accumulates with τ according to the following functions, shown in Figures 41 and 42: Brittle Damage Figure 41. Equation. Brittle damage small d of tau. Ductile Damage Figure 42. Equation. Ductile damage small d of tau. An alternative softening function is suggested in appendix A. The parameters A and B or C and D set the shape of the softening curve plotted as stressdisplacement or stressstrain. The parameter dmax is the maximum damage level that can be attained. It is set equal to approximately 1 in the tensile and low confining pressure regimes. Brittle damage is set to 0.999 to avoid computational difficulties associated with zero stiffness at a value of 1. At moderate confining pressures, it is less than 0.999, in agreement with TXE data with residual strength. It is set to less than 0.999 by the formula shown in Figure 43: Figure 43. Equation. Variation of dmax with stress invariant ratio. The power 1.5 was chosen by the developer based on examination of single element simulations and could be included as a usersupplied input parameter at a later date. The maximum damage level also varies with rate effects, as shown in Figure 44. The nondimensional term in parentheses is a stress invariant ratio that is equal to 1 in unconfined compression and less than 1 for stress states with confinement, as shown in Figure 45. Figure 44. Equation. Variation of dmax with rate effects. Figure 45. Schematic representation of four stress paths and their stress invariant ratios. In addition to reducing the maximum damage level with confinement (pressure), the compressive softening parameter, A, may also be reduced with confinement. The formulation is shown in Figure 46: Figure 46. Equation. Reduction of A with confinement. Here pmod is a userspecified input parameter. Its default value is 0.0. Input positive value of pmod reduces A when the maximum damage is less than 0.999; otherwise A is unaffected by pmod. Thus, it is only active at moderate confinement levels. The maximum increment in damage that can accumulate over a single time step is 0.1 (10 percent). This maximum increment is set internally to avoid excessive damage accumulation over a single time step. Excessive damage accumulation can lead to unstable behavior. This 0.1 damage increment was chosen by the developer based on examination of numerous multielement simulations and could be included as a usersupplied input parameter at a later date. Regulating Mesh Size Sensitivity. If the equations shown in Figure 41 and Figure 42 are used as is to model softening, the softening behavior would be mesh size dependent. This behavior means that different mesh refinements would produce different computational results, typically with the greatest damage accumulation in the smallest elements. This behavior is undesirable and is the result of modeling smaller fracture energy in the smaller elements. The fracture energy is the area under the stressdisplacement curve in the softening regime. Direct use of the equations shown in Figure 41 and Figure 42 is demonstrated in the concrete model evaluation report for direct pull and unconfined compression of concrete cylinders.^{(1)} The calculations without softening regulation demonstrate that convergence of the solution is not attained as the mesh is refined to a reasonable element size of about 19 to 38 millimeters (mm) (0.75 to 1.5 inches) for concrete. It is desirable for a computational solution to converge as the mesh is refined. Regulatory methods promote convergence by reducing or eliminating elementtoelement variation in fracture energy. The fracture energy is a property of a material, and special care must be taken to treat it as such. Several possible approaches are available for regulating mesh size dependency. One approach is to manually adjust the damage parameters as a function of element size to keep the fracture energy constant. However, this approach is not practical because the user would need to input different sets of damage parameters for each size element. A more automated approach is to include an element length scale in the model. This is done by passing the element size through to the material model and internally calculating the damage parameters as a function of element size. Finally, viscous methods for modeling rate effects have also been proposed (in the literature) to regulate mesh size dependency. However, if rateindependent calculations are performed, then viscous methods will be ineffective. To regulate mesh size sensitivity, the concrete model maintains constant fracture energy regardless of element size. This is done by including the element length, L (cube root of the element volume), and a fracture energy type term, G_{f} , in the softening parameter A of the equation in Figure 41, or C of the equation in Figure 42. The most general way to maintain constant fracture energy is to derive an expression for the fracture energy by integrating the analytical stressdisplacement curve as shown in Figure 47: Figure 47. Equation. Fracture energy integral for G_{f}. Here x is the displacement and x_{0} is the displacement at peak strength, f¢ . The fracture energy is defined in terms of the damage softening parameters (with dmax = 1) and element length by substituting either damage formulation (equations in Figure 41 or in Figure 42) into and performing the integration. To accomplish the integration, the damage threshold difference (τ  r_{0}) must be specified. The damage threshold difference is dependent on whether brittle or ductile damage is modeled. Brittle softening (P < 0) and ductile softening (P > 0) are regulated separately, because brittle damage accumulation is modeled differently from ductile damage accumulation. For brittle damage, the relationship between the fracture energy, G_{f}, the softening parameters, C and D, the initial damage threshold, r_{0b}, and element size, L, is shown in Figure 48: Figure 48. Equation. Brittle damage fracture energy G_{f}. This expression was obtained by integrating the equation in Figure 47 using the definition of the damage threshold difference shown in Figure 49: Figure 49. Equation. Brittle damage threshold difference τ minus small r_{0b}. Rearranging the equation in Figure 48 gives the softening parameter C shown in Figure 50: Figure 50. Equation. Brittle softening parameter C. For ductile damage, the relationship between the fracture energy, G_{f}, the softening parameters, A and B, the initial damage threshold, r_{0d}, and element size, L, is shown in Figure 51: Figure 51. Equation. Ductile damage fracture energy G_{f}. This expression was obtained by integrating the equation in Figure 47 using the definition of the damage threshold difference shown in Figure 52: Figure 52. Equation. Ductile damage threshold difference τ − r_{0d}. The integral on the right of the equation in Figure 51 reduces to a dilogarithm, which is not solvable in closed form. Therefore, its value is internally calculated by the LSDYNA concrete model during the initialization phase. Its value depends on the input parameter B and is termed dilog. Rearranging the equation in Figure 51 gives the softening parameter A shown in Figure 53: Figure 53. Equation. Ductile softening parameter A. In summary, to regulate mesh size dependency, the concrete model requires input values for B and G_{fc} rather than for A and B. Similarly, the concrete model requires input values for D and G_{ft} rather than for C and D. When the brittle damage threshold is attained, the concrete material model internally solves the equation in Figure 48 for the value of A based on the initial element size, the initial brittle damage threshold, the brittle fracture energy, and a userspecified input value for B. When the ductile damage threshold is attained, the concrete material model internally solves the equation in Figure 51 for the value of C based on the initial element size, the initial ductile damage threshold, and the ductile fracture energy, and a userspecified input value for D. Refer to the concrete model evaluation report, which discusses cylinder compression calculations conducted with regulation of the softening response.^{(1)} The calculations conducted in tension demonstrate that brittleness increases with mesh refinement until convergence is attained. Conversely, the calculations conducted in compression demonstrate that brittleness decreases with mesh refinement until convergence is attained. Specifying the Fracture Energy. The user specifies three distinct fracture energy values. These are the fracture energy in uniaxial tensile stress, G_{ft}, pure shear stress, G_{fs}, and uniaxial compressive stress, G_{fc.} The model internally selects the brittle or ductile fracture energy from equations that interpolate between the three fracture energy values as a function of the stress state. The stress state is defined by a nondimensional stress invariant ratio call trans. The interpolation is as shown in Figures 54 and 55: Figure 54. Equation. Brittle damage threshold G_{f} ^{Brittle}. Figure 55. Equation. Ductile damage threshold G_{f} ^{Ductile}. Here trans is the interpolation parameter whose value ranges between 0 in pure shear stress to 1 in uniaxial tensile or compressive stress. The interpolation depends on two userspecified input parameters. These are pwrt for the tensiletoshear transition and pwrc for the sheartocompression transition. Fracture Energy with Rate Effects. When rate effects are modeled with viscoplasticity, the user has the option to increase the fracture energy as a function of the rate effect. This is accomplished via the repow parameter as shown in Figure 56: Figure 56. Equation. The fracture energy with rate effects, G^{vp}_{f} . Here G_{f} is either the brittle or ductile fracture energy calculated from the userspecified input values, and is the value that is scaled up with rate effects. A value of repow = 1 is recommended. With a value of 1, the increase in fracture energy with rate effects is approximately proportional to the increase in strength with rate effects. With a value of repow = 0, constant fracture energy is maintained independent of rate effects. Refer to appendix B of the concrete model evaluation report for a review of calculations conducted with repow ranging between 0 and 1.^{(1)} They indicate that repow = 0 tends to model a response that is more brittle than measured in bridge rail impact tests. The recommended range is between 0.5 and 1. Tracking Damage. Two distinct damage parameters are tracked. One parameter is the ductile damage parameter, denoted d ^{d}. The ductile damage parameter increases in value whenever the ductile damage formulation is active (pressure is compressive) and τ exceeds the current damage threshold. The value of the ductile damage parameter never decreases, even temporarily. The other parameter is the brittle damage parameter d ^{b}. The brittle damage parameter increases in value whenever the brittle (pressure tensile) damage formulation is active and τ exceeds the current damage threshold. When inactive, the brittle damage parameter is temporarily set equal to zero in order to model stiffness recovery with crack closing. In other words, brittle damage drops to zero (stiffness is recovered) whenever the pressure switches from tensile to compressive. The maximum value of d ^{b} is recovered when the brittle formulation becomes active again (when the pressure becomes tensile again). A userspecified input parameter, called recov, is available to control stiffness recovery. It is by default zero, which means 100 percent recovery of stiffness and strength when pressure becomes compressive. A value of 1 would provide no recovery of stiffness and strength; hence brittle damage remains at its maximum level. Values between 0 and 1 model partial recovery. Its implementation is shown in Figure 57: Figure 57. Equation. Default damage recovery of d of τ_{t} . The damage parameter applied to the six stresses is equal to the current maximum of the brittle or ductile damage parameter: d=max(d ^{b}, d ^{d}). An option is also available to control stiffness recovery as a function of volumetric strain as well as pressure, as shown in Figure 58: Figure 58. Equation. Optional damage recovery of d of τ_{t}. To select this option, recov is specified by the user with an initial value between 10 and 11, rather than between 0 and 1. When recov is 10 or greater, a flag is internally set to base stiffness recovery on volumetric strain as well as pressure. In addition, the concrete model internally subtracts 10 from recov to obtain a value between 0 and 1 for use in the above formulation. Element Erosion. An element loses all strength and stiffness as d® 1. To prevent computational difficulties, such as mesh tangling and shooting nodes, element erosion is available as a user option. An element erodes when d > 0.99 and the maximum principal strain is greater than a usersupplied input value. Rate Effects FormulationRate effects formulations are implemented to model an increase in strength with increasing strain rate such as that previously shown in Figure 13. The rate effects formulations are applied to the plasticity surface, the damage surface, and the fracture energy. This section discusses rate effects as they apply to the plasticity surface. Rate effects as they apply to the damage surface and fracture energy were previously discussed in the section on damage formulation above. Viscoplastic Formulation. The viscoplastic algorithm is applied to the yield surface. The implementation is based on the Simo et al. extension of the commonly used DuvautLions formulation to cap models.^{(26)} The Simo et al. extension requires one rate effects parameter, denoted by η. This parameter is called the fluidity coefficient and is a userspecified input parameter. The basic viscoplastic update algorithm is simple to implement. At each time step, the algorithm interpolates between the elastic trial stress and the inviscid stress (without rate effects) to set the viscoplastic stress (with rate effects), as shown in Figure 59: Figure 59. Equation. Viscoplastic stress update for σ^{vp}_{ij}. This interpolation depends on the fluidity coefficient, η, and the time step, Δt. When η = 0, the inviscid stress is attained so that the solution is independent of strain rate. As η ® ¥, the elastic trail stress is attained at each and every time step. This corresponds to the absence of plastic flow. Therefore, plastic flow decreases as rate effects increase. At each time step, the viscoplastic stress is bounded between the current rateindependent stress and the elastic trial stress. The viscoplastic algorithm allows the viscoplastic stress state to lie outside the yield surface. The model's flexibility in fitting high strain rate data is improved by converting the single parameter viscoplastic formulation to a twoparameter formulation. This is a simple modification, shown in Figure 60, in which:^{(27)} Figure 60. Equation. Twoparameter η. The two input parameters are η_{0} and n. The user can fit rate effects data at two strain rates, instead of at one strain rate, which provides a better fit to the data. The behavior modeled by the viscoplastic update for direct pull and unconfined compression simulations is as shown in Figure 61: Figure 61. Equation. Dynamic strengths, f ′_{T} ^{dynamic}, and f ′_{C} ^{dynamic}. Here it is shown that the dynamic strength (viscoplastic) is equal to the static strength (inviscid) plus a dynamic overstress equal to E η where E is Young's modulus and is the effective strain rate. The effective strain rate depends on all six strain components as shown in Figure 62: Figure 62. Equation. Effective strain rate . The overstress modeled in tension is the same as that modeled in compression. This means that at high strain rates, the dynamictostatic strength ratio in tension is about a factor of 10 greater than the dynamictostatic strength ratio in compression, because the tensile strength is about onetenth the compressive strength. Hence, the viscoplastic model simulates larger rate effects in tension than in compression, consistent with the data trend previously shown in Figure 14. Viscoplastic Input. Although the basic two parameter formulation models more significant rate effects in tension than compression, the user may still wish to fit tensile and compressive strain rate data with different viscoplastic fluidity parameters. This is done with four userspecified input parameters. These are η_{0t} and n_{t} for fitting uniaxial tensile stress data, and a separate set, η_{0c} and _{c}, for fitting the uniaxial compressive stress data. For stress states between uniaxial tensile stress and uniaxial compressive stress, the fluidity parameter is interpolated as a function of stress invariant ratio. The interpolation is shown in Figures 63 and 64: Figure 63. Equation. Variation of fluidity parameter η in tension. Figure 64. Equation. Variation of fluidity parameter η in compression. Here, the effective η_{t} , η_{s} , and η_{c} are the fluidity parameters in uniaxial tensile stress, shear stress, and uniaxial compressive stress. They are determined from five input parameters as shown in Figure 65: Figure 65. Equation. Effective fluidity parameters, η_{t}, η_{c}, and η _{s}. The effective fluidity parameter in shear is determined from a single input scaling parameter, Srate. This viscoplastic model may predict substantial rate effects at high strain rates ( > 100). To limit rate effects at high strain rates, the user may input overstress limits in tension (overt) and compression (overc). These input parameters limit calculation of the fluidity parameter as shown in Figure 66: Figure 66. Equation. Overstress limit of η. where over = overt when the pressure is tensile, and over = overc when the pressure is compressive. Kinematic HardeningIn unconfined compression, the stressstrain behavior of concrete typically exhibits nonlinearity and dilation prior to the peak. This behavior was previously demonstrated in Figure 5 and Figure 10. This type of behavior is modeled with an initial shear yield surface, N_{H}F_{f} , which hardens until it coincides with the ultimate shear yield surface, F_{f}. Two input parameters are required. One parameter, N_{H}, initiates hardening by setting the location of the initial yield surface as a fraction of the final yield surface. Reasonable values are approximately 0.7 < N_{H} £ 1.0. A second parameter, C_{H}, determines the rate of hardening (amount of nonlinearity). The state variable that defines the translation of the yield surface is known as the back stress and is denoted by α_{ij}. The incremental backstress is Δα_{ij}. The value of each back stress component is zero upon initial yielding and reaches a maximum value at ultimate yield. The total stress is updated from the sum of the initial yield stress () plus the back stress (see Figures 67 and 68):Figure 67. Equation. Back stress α _{ij} ^{n} ^{+ 1}. Figure 68. Equation. Updated stress with hardening, σ^{P} _{ij} ^{n}^{+1}. The hardening rule defines the growth of the back stress. Hardening rules are typically based on stress or plastic strain. The model bases hardening upon stress to ensure that the translating shear surface coincides with the ultimate surface (lack of proper translation is a problem with plastic strain based rules). This process is accomplished by defining the incremental back stress, as shown in Figure 69: Figure 69. Equation. Incremental back stress, Δα_{ij}. Here C_{H} is the user input parameter that determines the rate of translation, G_{α} is a function that properly limits the increments, and  α_{ij} are the elastoplastic stress components that determines the direction of translation for each component. Also included in the formulation is the effective strain rate increment, , and the time step, Δt. These terms are internally calculated by the material model and LSDYNA, and are included to keep the hardening response independent of time step, time step scale factor, and strain increment. The input parameter C_{H} is the rate of translation used in unconfined compression. In the brittle regime (and for pure shear stress) the rate of translation is internally increased to 10C_{H}. For stress states with low confinement, the rate of translation transitions between the brittle value and the input value are shown in Figures 70 and 71: Figure 70. Equation. Brittle rate of translation C_{H} ^{Brittle}. Figure 71. Equation. Ductile rate of translation C_{H} ^{Ductile}. The function G_{α} restricts the motion of the yield surface so that it cannot translate outside the ultimate surface.^{(23)} The functional form of G_{α} is determined from the functional form of the yield surface. It is defined as shown in Figure 72: Figure 72. Equation. The limiting function G_{α.} The value of the limiting function is G_{α} = 1 at initial yield, because α_{ij} = 0 at initial yield. The value of the limiting function is G_{α} = 0 at ultimate yield, because the numerator equals the denominator (for the main term in brackets) at ultimate yield. Thus, G_{α} limits the growth of the back stress as the ultimate yield surface is approached. The developer has chosen to square the term in brackets based on review of the behavior of single element simulations. The square power could be replaced with a userdefined input parameter at a later date. Each term in the denominator warrants a verbal description. The term on the left is the value of the ultimate yield surface, evaluated at the pressure invariant with backstress (before application of damage and viscoplasticity). The term on the right is the value of the initial yield surface, evaluated at the pressure invariant without backstress (also before application of damage and viscoplasticity). Use of the kinematic hardening formulation modifies the shear surface definition, as shown in Figure 73: Figure 73. Equation. Modified shear failure surface, F_{f}. If kinematic hardening is not requested (C_{H} and N_{H} are set to zero), then the value of N_{H} is internally reset to 1.0. In this way, the original (ultimate) shear surface is recovered. Model InputEase of use is an important consideration for the roadside safety community. Many users have significant experience performing LSDYNA analyses, but they are less experienced in material modeling topics. Often, users lack the necessary time, data, and material modeling experience to accurately fit a set of material model parameters to data. The ability of a material model to simulate real world behavior not only depends on the theory of the material model, but on the fit of the material model to laboratory test data. The current version of concrete material model 159 has up to 37 input parameters, with a minimum of 19 parameters that must be fit to data. The model has been made easy to use by implementing a set of standardized material properties for use as default material properties. Default material model parameters are provided for the concrete model based on three input specifications: the unconfined compression strength (grade), the aggregate size, and the units. The parameters are fit to data for unconfined compression strengths between about 20 and 58 MPa (2,901 to 8,412 psi), with emphasis on the midrange between 28 and 48 MPa (4,061 and 6,962 psi). The unconfined compression strength affects all aspects of the fit, including stiffness, threedimensional yield strength, hardening, and damage. The fracture energy affects only the softening behavior of the damage formulation. Softening is fit to data for aggregate sizes between 8 and 32 mm (0.3 and 1.3 inches). The suite of material properties was primarily obtained through use of the CEBFIP Model Code.^{(11)} This code is a synthesis of research findings and contains a thorough section on concrete classification and constitutive relations. Various material properties, such as compressive and tensile strengths, stiffness, and fracture energy, are reported as a function of grade and aggregate size. 
Topics: research, infrastructure, pavement and materials Keywords: research, infrastructure, materials, Concrete, LSDYNA, Material model, Plasticity, Damage, Rate effects, Reinforced beam TRT Terms: Concrete–Mathematical models–Handbooks, manuals, etc, Finite element method Updated: 04/23/2012
